General

Property | Temperature | Value |
---|---|---|

Density | 23.0 °C | 2.65 - 2.7 g/cm³ Show Material materials with Density of 2.65 - 2.7 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Compressive modulus | 23.0 °C | 71.7 MPa Show Material materials with Compressive modulus of 71.7 MPa | |

Elastic modulus | 23.0 °C | 71 GPa Show Material materials with Elastic modulus of 71 GPa | |

Elongation | -195.0 °C | 36 % Show Material materials with Elongation of 36 % | Elongation in 50 mm |

-80.0 °C | 30 % Show Material materials with Elongation of 30 % | Elongation in 50 mm | |

0.0 °C | 27 % Show Material materials with Elongation of 27 % | Elongation in 50 mm | |

23.0 °C | 16 % Show Material materials with Elongation of 16 % | Elongation in 50 mm | |

24.0 °C | 25 % Show Material materials with Elongation of 25 % | Elongation in 50 mm | |

100.0 °C | 36 % Show Material materials with Elongation of 36 % | Elongation in 50 mm | |

150.0 °C | 50 % Show Material materials with Elongation of 50 % | Elongation in 50 mm | |

205.0 °C | 60 % Show Material materials with Elongation of 60 % | Elongation in 50 mm | |

260.0 °C | 80 % Show Material materials with Elongation of 80 % | Elongation in 50 mm | |

315.0 °C | 110 % Show Material materials with Elongation of 110 % | Elongation in 50 mm | |

370.0 °C | 130 % Show Material materials with Elongation of 130 % | Elongation in 50 mm | |

Elongation A100 | 23.0 °C | 10 - 20 % Show Material materials with Elongation A100 of 10 - 20 % | |

Elongation A50 | 23.0 °C | 14 - 16 % Show Material materials with Elongation A50 of 14 - 16 % | |

Fatigue strength | 23.0 °C | 160 MPa Show Material materials with Fatigue strength of 160 MPa | for 5x10⁸ cycles |

Hardness, Brinell | 23.0 °C | 75 [-] Show Material materials with Hardness, Brinell of 75 [-] | |

Plane-Strain Fracture Toughnes | 23.0 °C | 22 - 35 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 22 - 35 MPa·√m | Typical for Wrought 5000 Series Aluminium |

Poisson's ratio | 23.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | Typical for Wrought 5000 Series Aluminium |

Shear modulus | 23.0 °C | 26.4 GPa Show Material materials with Shear modulus of 26.4 GPa | |

Shear strength | 23.0 °C | 172 MPa Show Material materials with Shear strength of 172 MPa | |

Tensile strength | -195.0 °C | 407 MPa Show Material materials with Tensile strength of 407 MPa | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture |

-80.0 °C | 295 MPa Show Material materials with Tensile strength of 295 MPa | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |

0.0 °C | 290 MPa Show Material materials with Tensile strength of 290 MPa | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |

23.0 °C | 125 - 350 MPa Show Material materials with Tensile strength of 125 - 350 MPa | ||

24.0 °C | 290 MPa Show Material materials with Tensile strength of 290 MPa | ||

100.0 °C | 275 MPa Show Material materials with Tensile strength of 275 MPa | ||

150.0 °C | 215 MPa Show Material materials with Tensile strength of 215 MPa | ||

205.0 °C | 152 MPa Show Material materials with Tensile strength of 152 MPa | ||

260.0 °C | 117 MPa Show Material materials with Tensile strength of 117 MPa | ||

315.0 °C | 75 MPa Show Material materials with Tensile strength of 75 MPa | ||

370.0 °C | 40 MPa Show Material materials with Tensile strength of 40 MPa | ||

Unlock all property charts | |||

Yield strength | 23.0 °C | 140 MPa Show Material materials with Yield strength of 140 MPa | |

Yield strength Rp0.2 | -195.0 °C | 165 MPa Show Material materials with Yield strength Rp0.2 of 165 MPa | |

-80.0 °C | 145 MPa Show Material materials with Yield strength Rp0.2 of 145 MPa | ||

-30.0 °C | 145 MPa Show Material materials with Yield strength Rp0.2 of 145 MPa | ||

23.0 °C | 100 - 200 MPa Show Material materials with Yield strength Rp0.2 of 100 - 200 MPa | ||

25.0 °C | 145 MPa Show Material materials with Yield strength Rp0.2 of 145 MPa | ||

100.0 °C | 145 MPa Show Material materials with Yield strength Rp0.2 of 145 MPa | ||

150.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | ||

205.0 °C | 115 MPa Show Material materials with Yield strength Rp0.2 of 115 MPa | ||

260.0 °C | 75 MPa Show Material materials with Yield strength Rp0.2 of 75 MPa | ||

315.0 °C | 50 MPa Show Material materials with Yield strength Rp0.2 of 50 MPa | ||

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 20.0 °C | 2.38E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.38E-5 1/K | |

23.0 °C | 2.4E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.4E-5 1/K | ||

100.0 °C | 2.38E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.38E-5 1/K | ||

Unlock all property charts | |||

Max service temperature | 150 °C Show Material materials with Max service temperature of 150 °C | Typical for Wrought 5000 Series Aluminium | |

Melting point | 570 - 640 °C Show Material materials with Melting point of 570 - 640 °C | ||

Specific heat capacity | 23.0 °C | 900 J/(kg·K) Show Material materials with Specific heat capacity of 900 J/(kg·K) | |

Thermal conductivity | 23.0 °C | 117 - 121 W/(m·K) Show Material materials with Thermal conductivity of 117 - 121 W/(m·K) |

Electrical

Property | Temperature | Value | Comment |
---|---|---|---|

Electrical conductivity | 23.0 °C | 1.70E+7 S/m Show Material materials with Electrical conductivity of 1.70E+7 S/m | Typical value |

Electrical resistivity | 23.0 °C | 5.8E-8 - 6E-8 Ω·m Show Material materials with Electrical resistivity of 5.8E-8 - 6E-8 Ω·m | Typical value |

Specific Electrical conductivity | 29 % IACS Show Material materials with Specific Electrical conductivity of 29 % IACS | Typical/Derived value |

Chemical properties

Property | Value | Comment |
---|---|---|

Aluminium | 92.4 - 95.6 % Show Material materials with Aluminium of 92.4 - 95.6 % | Balance |

Chromium | 0.05 - 0.25 % Show Material materials with Chromium of 0.05 - 0.25 % | |

Copper | 0 - 0.1 % Show Material materials with Copper of 0 - 0.1 % | Typical |

Iron | 0 - 0.4 % Show Material materials with Iron of 0 - 0.4 % | |

Magnesium | 4 - 4.9 % Show Material materials with Magnesium of 4 - 4.9 % | |

Manganese | 0.4 - 1 % Show Material materials with Manganese of 0.4 - 1 % | |

Other | 0 - 0.15 % Show Material materials with Other of 0 - 0.15 % | each 0.05, total 0.15, Rest Al,Total |

Silicon | 0 - 0.4 % Show Material materials with Silicon of 0 - 0.4 % | |

Titanium | 0 - 0.25 % Show Material materials with Titanium of 0 - 0.25 % | |

Zinc | 0 - 0.25 % Show Material materials with Zinc of 0 - 0.25 % |

Technological properties

Property | ||
---|---|---|

Application areas | Ship building, Rail cars, Vehicle bodies, Tip truck bodies, Mine skips and cages, Pressure vessels | |

Brazing | general: no brazing is known or developed | |

Corrosion properties | Stress corrosion cracking: kein Schadensfall im Betrieb und bei Labortests (O, H321, H116), kein Schadensfall im Betrieb, eingeschränkte Schäden bei den Labortests (H111), general: very good, without protection in industrial or seawater atmosphere | |

General machinability | General: poor | |

Soldering general | Poor | |

Welding | When welding 5083 to itself or another alloy from the same sub-group, the recommended filler metal is 5183. Other suitable fillers are 5356 and 5556. Gas: Average; Arc: Excellent; Resistance: Excellent | |

Workability | general (condition): acceptable (O), poor(H321, H116, H111) |